Korean J. Chem. Eng., 21(2), 430-435 (2004)
†To whom correspondence should be addressed.
‡This paper is dedicated to Professor Hyun-Ku Rhee on the occasion
of his retirement from Seoul National University.
Photocatalytic Decolorization of Rhodamine B by Fluidized Bed Reactor
with Hollow Ceramic Ball Photocatalyst
Young-Soo Na, Do-Han Kim, Chang-Han Lee, Song-Woo Lee, Young-Seek Park*,
You-Kwan Oh, Sung-Hoon Park and Seung-Koo Song†
Department of Chemical Engineering, Pusan National University, Jangjeon-dong, Geumjeong-gu, Busan 609-735, Korea
*Department of Environmental Hygiene, Daegu University, Daegu 705-714, Korea
(Received 8 September 2003 • accepted 2 January 2004)
Abstract−−−−Photocatalytic degradation of organic contaminants in wastewater by TiO2 has been introduced in both
bench and pilot-scale applications in suspended state or immobilized state on supporting material. TiO2 in suspended
state gave less activity due to its coagency between particles. Recent advances in environmental photocatalysis have
focused on enhancing the catalytic activity and improving the performance of photocatalytic reactors. This paper reports
a preliminary design of a new immobilized TiO2 photocatalyst and its photocatalytic fluidized bed reactor (PFBR) to
apply photochemical degradation of a dye, Rhodamine B (RhB). But it was not easy to make a cost-effective and well
activated immobilized TiO2 particles. A kind of photocatalyst (named Photomedium), consisting of hollow ceramic
balls coated with TiO2-sol, which was capable of effective photodegradation of the dye, has been presented in this study.
The photocatalytic oxidation of RhB was investigated by changing Photomedia concentrations, initial RhB concen-
trations, and UV intensity in PFBR.
Key words: Photocatalyst, Fluidized Bed, Immobilization, TiO2, Toxicity
Industrial development is pervasively connected with the dis-
posal of number of toxic pollutants that are harmful to the environ-
ment and the human and are also not easily degraded in nature. In
particular, the wastewater from a textile dyeing process contains
numerous concentrated organic compounds that are toxic and col-
orful, which causes ineffectiveness of biological treatment [Nigam
et al., 1996]. Photocatalytic treatment is an attractive alternative,
since it does not need oxidants and does not produce secondary pol-
lutants [Ollis et al., 1991]. The mechanism of the photocatalytic ox-
idation of organic contaminants by TiO2 has been studied and ex-
plained by the band gap energy model [Turchi et al., 1990]. When
Ultraviolet (UV) illumination irradiates energy (λ
Photocatalytic Decolorization of RhB by Fluidized Bed Reactor with Hollow Ceramic Ball Photocatalyst 431
1-1. Rhodamine B (RhB)
The dye, RhB (reagent grade, 95% pure) is used as a test pol-
lutant. Its structure is given in Fig. 1. The RhB is sold as a green
crystal or a reddish-violet powder. It is highly soluble in water and
organic solvent and its molecular formula is C28H31CN2O3 (mol wt
479.00). Its color is fluorescent bluish-red. The RhB has been used
as a dye especially for paper and as a biological stain. But, the RhB
has been found to be a potentially toxic and carcinogenic substance.
This compound is now banned for food and cosmetic usages [Merck
The Photomedia were prepared by following procedures. Zeo-
lite, glass and TiO2 powder were mixed with silicone sealant. The
mixture was coated onto the surface of the EPS (Expandable Poly-
styrene) with mean diameter of 1.4 mm and was dried at room tem-
perature in a dust-free environment for 24 hours. Then, the EPS
ball was calcinated at 800-1,100oC in furnace for 4-8 hours to form
a hollow ceramic ball. The hollow ceramic ball was dipped into a
colloidal suspension (TiO2 sol: TiO2 content 1%, Deiha-international,
Korea) for 1 minute and dried at room temperature in a dust-free
environment for 24hours, then calcinated at 500oC in air for 2hours.
The average diameter of the Photomedia was about 1.5 mm and
the thickness, approximately 65µm (Fig. 4).
The specific design of PFBR (Fig. 2) was as follows. Four 20 W
UV lamps (Sankyo Denki) were installed inside the reactor (Vol-
ume; 24 L). The vertical plate inside the reactor and the air stream
blowing from the bottom of the reactor at the rate of 1 L/min help-
ed make it possible for Photomedia and reactants to be well fluid-
ized and mixed perfectly.
1-4. Analysis of Data
The spectrophotometer (Lambda 20: PERKIN ELMER) was used
for analyzing optical absorption spectra of degraded RhB solution.
The maximum adsorption wavelength was found to be 550nm. The
RhB concentration was calculated by the calibration curve of RhB
concentration at wavelength of 550 nm.
The hardness of the Photomedium was measured by DMA (Dy-
namic Mechanical Analyzer). Oxygen, silicon and titanium ele-
ments of the surfaces of the Photomedia were measured by the SEM/
EDX analyzer (HITACHI S-4200, Japan).
EC50 is the effluent concentration that causes a measurable n
tive effect on 50 percent of the test population. EC50 was investi-
gated to evaluate the toxicity of RhB and its reaction intermedia
This was determined by Microtox Toxicity Screening Test Syst
(Microtox M500) using Vibrio fischeri as a test microorganism.
RESULTS AND DISCUSSION
1. Hardness of Photomedium
Sintering time and temperature were varied to find an optim
condition for durable Photomedia. Fig. 3(a) and (b) show the h
ness of the Photomedia. The Photomedia incinerated at 800oC were
so fragile that their hardness was unmeasurable. When incine
at 1,100oC, the particles melted. The Photomedia prepared b
with/without TiO2 powder had a maximum value in hardness wh
incinerated at 900-1,000oC. At the temperatures of 900oC and 1,000
oC (except 5 hours), the hardness of the Photomedia premixed
TiO2 powder were approximately twice higher than those witho
Calcination temperature of 900oC for 6 hours with TiO2 powder
showed the highest value of hardness.
2. Effect of the Number of Coating with TiO2-sol
Fig. 2. The schematic diagram of PFBR.
Fig. 3. The effect of sintering time on the hardness of the Pho-
(a) 900oC, � without TiO2; � with TiO2
(b) 1,000oC, � without TiO2; � with TiO2
Korean J. Chem. Eng.(Vol. 21, No. 2)
432 Y.-S. Na et al.
The preparation process of the TiO2 coated hollow ceramic ball
was previously explained in detail [Na et al., 2001]. The analysis
of the EDX showed that the Photomedium has oxygen and silicon
on its surface along with a small amount of potassium and calcium
The effect of the numbers of coating with TiO2-sol on dye decom-
position was investigated with the initial concentration of the RhB,
6.8µM. Fig. 5 showed that the decrease of RhB concentration was
steepened according to the number of coatings up to three times.
But, from the quadruple coating, there was no remarkable decrease
of the RhB concentration and showed similar decreasing trend of
the triple coating. Although the surface coverage of TiO2 on the Pho-
tomedia increased with the number of coatings, the increase was
significant up to triple coating and no remarkable increase was shown
with further coatings.
Fig. 6 showed SEM photographs of the Photomedia with the n
ber of coatings. The Photomedium without coating by TiO2-sol [Fig.
6(a)] showed flat surface, whereas titania particles in the coated
ples were well distributed on the surface of the supporting mate
with nanometer size. When the surface coverage of TiO2 was com-
pared in Fig. 6(b) and Fig. 6(c), the content of titania on surface
the sixfold coated Photomedium was a little higher than that of
triple coated one, but titania layer of the sixfold coated Photom
dium was thicker than that of the triple-coated one due to the o
lap of TiO2 particles.
From the analysis of the Photomedia by EDX and SEM, it w
found that the titanium atom showed rapid spread until triple co
ing, but there was no significant increase after quadruple coatin
was considered that formation of multiple layers especially m
than 4 times did not alter the density of TiO2 active site on its sur-
This result suggested that the optimum number of coating w
for the decomposition of RhB. Therefore, all of the Photome
used in next experiments were fixed at triple coating.
Fig. 4. The SEM photograph of Photomedia (×40).
Table 1. Atomic composition (%) of the surface of the Photome-
0 1 2 3 4 5 6
O 67.83 67.83 63.41 65.03 67.10 68.78 58.32
Si 24.04 21.82 20.00 13.9709.31 07.18 11.61
Ti 00.00 10.35 16.60 21.01 23.59 24.04 30.07
Fig. 5. The effects of reaction time on the decolorization of RhB
(number of TiO2-sol coating; � one, � two, � three, �
four, � five, � six, � seven).
Fig. 6. The SEM photography of Photomedium (×100,000).
(a) no coating, (b) triple coating, (c) six-time coating
Photocatalytic Decolorization of RhB by Fluidized Bed Reactor with Hollow Ceramic Ball Photocatalyst 433
3. Effect of Photomedia Dosages
Since the photocata